| ||Format||Pages||Price|| |
|6||$45.00||  ADD TO CART|
|Hardcopy (shipping and handling)||6||$45.00||  ADD TO CART|
|Standard + Redline PDF Bundle||12||$54.00||  ADD TO CART|
Significance and Use
4.1 Since solar radiation, air temperature, relative humidity, and the amount and kind of atmospheric contaminants vary continuously, results from exposures based on elapsed time may differ. The variations in the results may be minimized by timing the exposures in terms of:
4.1.1 One or more environmental parameters such as solar radiant exposure, or
4.1.2 A predefined property change of a weathering reference specimen with known performance.
4.2 Variations in temperature, moisture and atmospheric contaminants can have a significant effect on the degradation caused by solar radiation. In addition, exposures conducted at different times of the year can cause large differences in rate of degradation. Different materials may have different sensitivities to heat, moisture, and atmospheric contaminants, which may explain differences in rankings of specimens exposed to equivalent solar radiant exposure when other environmental conditions vary.
4.3 Since the method of mounting may influence the temperature and other parameters during exposure of the specimen, there should be a mutual understanding as to the method of mounting the specimen for the particular exposure test under consideration.
4.4 There can be large differences among various single strength window glasses in their transmittance in the 300 to 350 nm region. For example, at 320 nm, the percent transmittance for seven different lots of single strength window glass ranged from 8.4 to 26.8 %. At 380 nm, the percent transmittance ranged from 84.9 % to 88.1 %.6
4.5 Differences in UV transmittance between different lots of glass persist after solarization. The largest differences among window glasses in UV transmittance are in the spectral range of 300 to 320 nm.
4.6 This practice is best used to compare the relative performance of materials tested at the same time behind the same lot of glass. Because of variability between lots of glass and between exposures conducted at different times of the year, comparing the amount of degradation in materials exposed for the same duration or radiant exposure at separate times, or in separate fixtures using different lots of glass is not recommended.
4.7 It is strongly recommended that at least one control material be exposed with each test. The control material should be of similar composition and construction. and be chosen so that its failure modes are the same as that of the material being tested. It is preferable to use two control materials, one with relatively good durability, and one with relatively poor durability. If control materials are included as part of the test, they shall be used for the purpose of comparing the performance of the test materials relative to the controls.
1.1 This practice evaluates the resistance of nonmetallic materials to solar radiation filtered through glass in passively ventilated and non-vented enclosures. For exposures in under glass enclosures with forced air circulation, refer to Practice G201.
1.2 For direct exposures, refer to Practice G7.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C1036 Specification for Flat Glass
D3424 Practice for Evaluating the Relative Lightfastness and Weatherability of Printed Matter
D4303 Test Methods for Lightfastness of Colorants Used in Artists Materials
D6901 Specification for Artists Colored Pencils
E824 Test Method for Transfer of Calibration From Reference to Field Radiometers
E903 Test Method for Solar Absorptance, Reflectance, and Transmittance of Materials Using Integrating Spheres
E1084 Test Method for Solar Transmittance (Terrestrial) of Sheet Materials Using Sunlight
G7 Practice for Atmospheric Environmental Exposure Testing of Nonmetallic Materials
G113 Terminology Relating to Natural and Artificial Weathering Tests of Nonmetallic Materials
G173 Tables for Reference Solar Spectral Irradiances: Direct Normal and Hemispherical on 37 Tilted Surface
G177 Tables for Reference Solar Ultraviolet Spectral Distributions: Hemispherical on 37 Tilted Surface
G201 Practice for Conducting Exposures in Outdoor Glass-Covered Exposure Apparatus with Air Circulation
ICS Number Code 59.080.01 (Textiles in general)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM G24-13, Standard Practice for Conducting Exposures to Daylight Filtered Through Glass, ASTM International, West Conshohocken, PA, 2013, www.astm.orgBack to Top